Investigation on Effect of Fiber and Orientation on the Properties of Bio-Fibre Reinforced Laminates
International Journal of Engineering Inventionse-ISSN: 2278-7461, p-ISSN: 2319-6491Volume 2, Issue 2 (January 2013) PP: 65-70www.ijeijournal.com P a g e | 65Investigation on Effect of Fiber and Orientation on theProperties of Bio-Fibre Reinforced LaminatesSripathy Malaiah1, Krishna Vinayak Sharma1, M Krishna21Department of Mechanical Engineering, UVCE, Bangalore University, KR Circle, Bangalore560001, India2Research and Development, R V College of Engineering, Mysore Road,Bangalore-560059, IndiaAbstract:- The objective of this work is to investigate the effect of fibre type and fibre orientation tensile andflexural shear properties of woven jute and bamboo fibre reinforced epoxy composites by experimentally.Laminates were fabricated by hand lay-up technique in a mould and cured under light pressure for 60 minfollowed by curing at room temperature for two days. Jute and bamboo laminates were made with a total of sixpiles by varying two orientation of fibre as to obtain four different samples. Specimen preparation and testingwas carried out as per ASTM standards. The results shows the tensile strength and flexural strengths of the juteand bamboo laminates higher at 0/90 orientation and jute shows the highest in both tensile and bendingstrength.Keywords:- Natural fibre, fibre orientation, tensile strength, SEM.I. INTRODUCTIONThe natural fibre reinforced composites (NFRC) are rapidly replacing petroleum based composites indifferent areas such as automotive, electrical construction and even building industries [1-3] due to low-densitymaterials yielding relatively light weight composites with high specific properties[4-5]. One of the mainimportant aspects of the behaviour of NFRC is their response to an bending load and the capacity of thecomposites to withstand it during their service life. Some of the reported work has suggested that NFRC arevery sensitive to impact loading .However the mechanical properties of natural fibre composites much lower than those of syntheticfibre composites . The fibre type and fibre orientation also influence on mechanical properties of NFRC.The aim of this work was to study the influence of fibre type and fibre orientation on the mechanical propertiesof epoxy composites and also studied fibre breakage during the experimental studies.II. EXPERIMENTAL STUDYCalcium hypochlorite and hydrogen peroxide used as a oxidizing agent to remove dust and oil fromnatural fibre. Alkanline treatement with NaOH, known as mercerization, extracts lignin and hemicelluloses,increasing the tensile strength and the elongation at break of the composite. In this process the fibre areimmersed in 10 wt.% solution of NaOH for two hours, followed by continuous washing and drying at 100 C.The composites used in the study were virtually identical in every aspect bamboo / jute used was plain-woven fabric type. The bamboo or jute was coated with an emulsion based sizing agent to promote goodchemical adhesion with the resin matrix. The resin used in this study was epoxy (Ciba-Geigy, Araldite-LY 556and Amine Hardener HY 951 – The resin hardener ratio- 100:10). The specimens were fabricated using wethand layup process. Woven mat 2-D fibers [0/90] and [45/45] were used in the specimens. The number of fiberlayers was derived based on the resin: fiber proportion 50: 50 wt % in all the cases. The specimens were cured atroom temperature for two weeks as most of the materials for industrial applications are naturally cured, beforeexposing to experimental conditions. The edges of the panels were sealed using the matrix resin beforeexposing to the experimental conditioning. This was to prevent the moisture permeation through these sides.Mechanical properties such as ultimate tensile strength (UTS), Young’s modulus, Flexural strength(FS), Flexural modulus of fibre reinforced epoxy composites are computed from the test conducted usinguniversal testing machine (UTM) in accordance to ASTM standards. The Test specimen geometry as specifiedin the above standard for balance symmetric glass are, width 12.7 mm, length 208 mm and thickness 3 mm.The test specimen is positioned vertically in the grips of the testing machine. The grips are tightened evenly andfirmly to prevent any slippage. The samples are cut to the dimensions as per ASTM standards for flexuraltesting. The test specimen geometry as specified in the above standard for balanced symmetric glass fibrecomposites (0/90) are , width 12.7 mm, length 127 mm, thickness 6 mm. The test is conducted at a strain rate of0.5mm/minute.
Investigation on Effect of Fiber and Orientation on the Properties of…www.ijeijournal.com P a g e | 66III. RESULTS AND DISCUSSION3.1 Tensile Strength with fibre orientationThe strain–stress curves for jute and bamboo composites with fibre orientation of 0/90 and 45/45 areplotted in Fig. 1. From this figure, an increase in maximum tensile strength and a reduction in strain is observedwith an increase in jute reinforced plastic composites at 0/90 fibre orientation being prominent. This indicatesthat jute fibre is acts as reinforcement and also as an effective stress transfer constituent in the compositesystem. Composite with 0/90 fibre orientation has demonstrated a factor of improvement in tensile strengthwhen compared with the 45/45 fibre orientation. The maximum tensile strength of jute fibre composites is22.01 Mpa with a strain at ultimate strength of 2.1%. The same trend of higher tensile strength is observed incase of bamboo composites.Fig. 1: Typical stress–strain curve of jute and bamboo epoxy composites for different fiber orientationFig. 2 Maximum tensile stress of Jute and bamboo composites at different fibre orientationA comparison of tensile strength between jute and bamboo specimens with different fibre orientation ispresented in Fig. 2, 3 and 4. It can be seen that the tensile properties of jute composites compares well withthose of bamboo composites for 0/90 and 45/45 fibre orientation. The tensile strength of jute 0/900composites is 535% more than that of jute 45/45, while jute 45/45 is 230% more than that of bamboo 0/90 andbamboo 0/90 is 191 % more than that of bamboo 45/45.The improved tensile strength in jute 0/90 could be attributed to several factors. Firstly, the density ofjute 0.88 g/cc is marginally less than that of bamboo matrix at 0.96 g/cc, which suggests that the jute has lessbranching, therefore providing stronger intermolecular forces and tensile strength.Secondly, during the recycling process the presence of additive compounds, such as cellouse, could improve thecompatibility of jute fibre with epoxy matrix, which in turn will increase the tensile strength of jute composites.With the 0/90 fibre orientation the maximum strength can be observed, the fibre matrix compatibility playsmore significant role in contributing mechanical properties of composites. As a consequence of this, themaximum tensile strength for jute composite with 0/90 fiber loading showed an improvement of nearly 6.53times when compared to that of jute with 45/45 orientation composites.
Investigation on Effect of Fiber and Orientation on the Properties of…www.ijeijournal.com P a g e | 67Fig.3: Strain (%) at maximum strength for jute and bamboo composites at different fibre orientationFig. 3 shows the values of strain at maximum strength and also as a function fibre orientation forcomposites containing both jute and bamboo composites. It can be observed here that there is improvement incomposite stiffness with an increase in fibre orientation in case of jute composites. However, in the case of thebamboo the reverse is observed. That is, the strain in the case of bamboo 45/45 orientation is higher thanbamboo with 0/90 orientation.Fig 6: Variation of flexural strength of jute and bamboo epoxy composites for different fiberorientationFig 7: Variation in strain at maximum bending strength for jute and bamboo epoxy composites atdifferent fiber orientationFig. 4 shows the results of the variation of Young’s Modulus (E) within the elastic limit as a functionof the fibre orientation for composites containing both jute and bamboo composites. As was observed in the caseof tensile strength, the value of Young’s Modulus can be seen to improve with an increase in fibre orientation. Asignificant improvement of the Young’s Modulus in the case of jute composites was observed at 0/90 fiberorientation when compared to that of 45/45 fiber orientation.3.2 Flexural Strength with fibre orientationFlexural strength, the strain at maximum strength and the flexural modulus at 1% and 3% strain for juteand bamboo composites were tested on the UTM in accordance with ASTM D790 standard. The dimensions ofthe test specimen were maintained to be as per the standard. Three specimens were tested in each case to ensurerepeatability of values.
Investigation on Effect of Fiber and Orientation on the Properties of…www.ijeijournal.com P a g e | 68Fig.4: Young’s modulus of jute and bamboo composites for different fibre orientationThe strain–stress curves for jute and bamboo composites with 45/45 and 0/90 fibre orientation areplotted and shown in Fig. 5. The figure shows an increase in maximum flexural strength and strain with anincrease in the angle of fibre orientation. This indicates that the jute fibre acts as a reinforcing and also as aneffective bending stress transfer constituent in the composite system.The flexural strength in the case of for both jute and bamboo composites laminates with 45/45 and0/90 fibre orientation are plotted and shown in Fig. 6. It can be observed that as the fibre orientation increases,there is an increase in the bending strength and stiffness. This is similar to the results obtained from testsconducted on tensile testing. The highest value of flexural strength and stiffness are seen in the case of jutecomposites laminates with 0/90 fiber orientation.The percentage decrease in the maximum flexural strength between Jute 0/90 to Jute 45/45 is a 217%and from jute 45/45 to bamboo 0/90 shows an increase in flexural strength by 14.91%.However there is adecrease in the maximum flexural strength from bamboo 0/90 to bamboo 45 by a factor of 94.12%.Thus the best orientation and composition is terms of the maximum flexural strength is 0/90 jutecomposite system with maximum flexural strength being 82.02 Mpa.However, in the case of bamboo composites laminates at 0/90 orientation, the bending strength and themodulus at 1% strain are 44.59 MPa and 685 Mpa, respectively. This could be attributed to the insufficientinterface bonding between fibers with epoxy matrix to transfer shear strength. In this study, the strain atmaximum flexural strength and the flexural modulus of composites at 1% and 3% strain are presented in Figures6.7, 6.8 and 6.9 respectively for the selected composite systems. This was done to specifically evaluate the lowflexural strain behaviour and stiffness for possible structural applications.The testing results indicate that jute/epoxy combination at 0/90 fiber orientation is the optimizedcombination for obtaining high flexural strength and modulus. The maximum bending strength and stiffness wasobserved for composites with 0/90 fiber orientation. This may be due to the higher compatibility and betterinterface bonding between the jute fibers and epoxy matrix. A summary of the flexural testing results arepresented in grahps. Results from both tensile and flexural testing results indicate that under quasi-static loadingcondition, the mechanical properties of the jute composites with epoxy matrix are compatible with those ofbamboo/epoxy matrixIV. FIBER FRACTURE AND DAMAGE STUDIESFig. 8: Variation of flexural modulus at 1% strain for jute and bamboo epoxy composites at different fiberorientation
Investigation on Effect of Fiber and Orientation on the Properties of…www.ijeijournal.com P a g e | 69Fig. 9: Variations of flexural modulus at 3% strain for jute and bamboo epoxy composites at different fiberorientationFig. 10 SEM image of fracture surface of a) Jute / epoxy composites laminates (0/90 fiber orientation), b) Jute /epoxy composites laminates (45/45 fiber orientation) c) bamboo/ epoxy composites laminates (0/90 fiberorientation), b) bamboo / epoxy composites laminates (45/45 fiber orientation)Fig. 10 shows an overview of the fractured surfaces of jute-epoxy (0/90 fibre orientation), jute-epoxy(45/45 fibre orientation), bamboo-epoxy (0/90 fibre orientation) and bamboo- epoxy (45/45 fibreorientation) composites. It shows many fibre pullouts in all composites and that bamboo fibres are coarser whencompared to jute fibres. Jute fibres are the thinnest when compared with the other and are also more evenlydistributed in the epoxy. The reason for this separation is expected to lie in the enzymatic retting process and thelower lignin content when compared with other fibres. Jute fibres are better dispersed and distributed in theepoxy matrix when compared with bamboo. Good dispersion and distribution of fibres is very important formechanical properties. It is also possible to see that in all the composites the fibre surfaces are clean whichindicates poor adhesion between the fibres and the matrix.V. CONCLUSIONThe objective of this study was to investigate effect of fibre and orientation affects the mechanicalproperties of NFRC. The tensile and bending strength were highest with jute fibre orientation of 0/90. This isbelieved to depend on fibre toughness along fibre pullouts. The electron microscopy study showed that bamboofibres were several times coarser than jute after processing. Furthermore jute fibres were separated to singleelementary fibres during the tested but bamboo fibres were still in the form of fibre bundles after processing.REFERENCES1) Karus M, Kaup M. Natural fibres in the European automotive industry. J Ind Hemp vol. 7 (2002),pp.117–29.2) Hepworth DG, Hobson RN, Bruce DM, Farrent JW. The use of unretted hemp fibre in compositemanufacture. Composites: Part A, vol. 31 (2000), pp1279–83.3) Jacob M, Thomas S, Varughese KT. Mechanical properties of sisal/ oil palm hybrid fibre reinforcednatural rubber composites. Compos Sci Technol, vol. 64 (2004), pp-955–65.4) Munawar SS, Umemura K, Kawai S. Characterization of the morphological, physical, and mechanicalproperties of seven nonwood plant fiber bundles. J Wood Sci, vol 53 (2007) pp.108–13.5) Brett S, William E. Natural fiber composites in automotive applications, in natural fiber composites inautomotive applications. CRC Press; 2005.
Investigation on Effect of Fiber and Orientation on the Properties of…www.ijeijournal.com P a g e | 706) Joshi SV, Drzal LT, Mohanty AK, Arora S. Are natural fiber composites environmentally superior toglass fiber reinforced composites? Compos A Appl Sci Manuf, vol. 35 (2004), pp.371–6.7) Ganster Johannes, Fink Hans-Peter. Novel cellulose fibre reinforced thermoplastic materials. Cellulose,vol. 13 (2006), pp.271–80.8) Maya JJ, Rajesh DA. Recent developments in chemical modification and characterization of naturalfiber reinforces composites. Polym Compos vo. 29 (2008) pp.187–207.M Sripathy, Obtained BE in Mechanical Engineering, ME in Manufacturing Science, andpursuing Ph.D in natural fiber sandwich structures, from UVCE, Bangalore University. His area of interest arenatural fiber sandwich structures, FRP, ect. He is active member of ISTE, He published number of papers inJournals.Krishna Vinayak Sharma obtained B.E, in Mech. Engg.,, ME in Design and Ph.D inComposites Materials form Bangalore University. At present he is Professor and Chairman of MechanicalEngineering, UVCE, Bangalore. He published 20 Journal publications in Journals. He successfully guided 2research Scholars for Ph.D’s. His research interest include: FEM, Composites, Sandwich etc.M Krishna BE, MS, Ph.D, is working as professor and Director, Research and Development, R VCollege of Engineering, Bangalore. He has published more than 100 research article in National andInternational Journals and presented more than 150 papers in National and International Conferences. Heexecuted more than 50 sponsored projects and consultancy.